Improved Photovoltaic Efficiency and Amplified Photocurrent Generation in Mesoporous n = 1 Two-Dimensional Lead‒Iodide Perovskite Solar Cells
Febriansyah, Benny; Koh, Teck Ming; Lekina, Yulia; Jamaludin, Nur Fadilah; Bruno, Annalisa; Ganguly, Rakesh; Shen, Ze Xiang; Mhaisalkar, Subodh G.; England, Jason; Chemistry of Materials 31 (2019) 890–; doi:10.1021/acs.chemmater.8b04064

data_4003078
_publ_section_title
;
 Improved Photovoltaic Efficiency and Amplified Photocurrent Generation in
 Mesoporous n = 1 Two-Dimensional Lead--Iodide Perovskite Solar Cells
;
_journal_issue                   3
_journal_name_full               'Chemistry of Materials'
_journal_page_first              890
_journal_paper_doi               10.1021/acs.chemmater.8b04064
_journal_volume                  31
_journal_year                    2019
_chemical_formula_sum            'C5 H9 I4 N3 Pb'
_chemical_formula_weight         825.94
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_update_record
;
2018-05-07 deposited with the CCDC.
2018-08-23 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 92.2131(7)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.8952(2)
_cell_length_b                   19.7237(5)
_cell_length_c                   8.9250(2)
_cell_measurement_reflns_used    9910
_cell_measurement_temperature    100.(2)
_cell_measurement_theta_max      33.1730
_cell_measurement_theta_min      2.2836
_cell_volume                     1564.69(6)
_computing_cell_refinement       'SAINT V8.38A (Bruker AXS Inc., 2017)'
_computing_data_collection       'APEX3 (Bruker AXS Inc., 2017)'
_computing_data_reduction        'SAINT V8.38A (Bruker AXS Inc., 2017)'
_computing_publication_material  'APEX3 (Bruker AXS Inc., 2017)'
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_structure_solution    'XS, VERSION 2013/1'
_diffrn_ambient_temperature      100.(2)
_diffrn_detector_area_resol_mean 7.4074
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'Photon II CPADs detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  'Multilayer Mirror'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0449
_diffrn_reflns_av_unetI/netI     0.0387
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       30
_diffrn_reflns_limit_k_min       -30
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            23604
_diffrn_reflns_theta_full        33.16
_diffrn_reflns_theta_max         33.16
_diffrn_reflns_theta_min         2.51
_diffrn_source                   'Incoatec microfocus source'
_diffrn_source_type              'Bruker D8 Quest'
_exptl_absorpt_coefficient_mu    18.647
_exptl_absorpt_correction_T_max  0.26
_exptl_absorpt_correction_T_min  0.04
_exptl_absorpt_correction_type   'Numerical Mu Calculated'
_exptl_absorpt_process_details
;
SADABS-2016/2 - Bruker AXS area detector scaling and absorption correction
;
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    3.506
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1416
_exptl_crystal_size_max          0.160
_exptl_crystal_size_mid          0.140
_exptl_crystal_size_min          0.100
_refine_diff_density_max         2.700
_refine_diff_density_min         -1.875
_refine_ls_extinction_coef       0.00264(11)
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_goodness_of_fit_ref   1.224
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     120
_refine_ls_number_reflns         5915
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.224
_refine_ls_R_factor_all          0.0310
_refine_ls_R_factor_gt           0.0300
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0159P)^2^+4.6832P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0717
_refine_ls_wR_factor_ref         0.0721
_reflns_number_gt                5754
_reflns_number_total             5915
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            cm8b04064_si_002.cif
_cod_data_source_block           (HA)[PbI4]
_cod_database_code               4003078
_shelx_res_checksum              8844
_shelx_hkl_checksum              1491